modern hybrid joints in aerospace modelling and
Post on 27-Jan-2016
Embed Size (px)
A R C H I V E S O F M E T A L L U R G Y A N D M A T E R I A L S
Volume 58 2013 Issue 1
T. SADOWSKI, T. BALAWENDER, R. LIWA, P. GOLEWSKI, M. KNE
MODERN HYBRID JOINTS IN AEROSPACE: MODELLING AND TESTING
NOWOCZESNE POCZENIA HYBRYDOWE W LOTNICTWIE: MODELOWANIE I BADANIA ESKPERYMENTALNE
The aim of the paper is to review different types of modern hybrid joints applied in aerospace. We focused on threeparticular cases: 1) spot welding adhesive, 2) rivet-bonded and 3) clinch-bonded joints. The numerical models presented inthe paper for these joints describe their complex behaviour under mechanical loading. The numerical calculations performedusing ABAQUS code were compared to experimental results obtained by application of the Digital Image Correlation system(DIC) ARAMIS.
The results investigated within the paper lead to the following major conclusions: the strengthening of joints by application of adhesive significantly improve static strength, the final failure of the joined structural system significantly depends on the surface adhesive area, the stiffening effects of the hybrid joint lead to higher reliability and durability of the structural joints.Keywords: clinching, hybrid joint, rivet-adhesive bonded joint, clinch adhesive joint, spot welding adhesive joint, FEA
(finite element analysis), DIC (digital image correlation system)
W pracy dokonano przegldu rnych typw pocze hybrydowych stosowanych w lotnictwie. Szczegln uwag zwr-cono na trzy typy pocze: 1) zgrzewanie punktowe klejenie, 2) nitowanie klejenie, 3) klinczowanie klejenie. Modelenumeryczne zczy zawarte w pracy, ujawniaj zoon i trudn do przewidzenia reakcj tych zczy na obcienia mechaniczne.Obliczenia numeryczne porwnano z wynikami eksperymentalnymi otrzymanymi za pomoc bezdotykowego systemu pomiaruodksztace i napre (DIC) ARAMIS.
Gwne wnioski z prezentowanych bada: zastosowanie kleju powoduje istotne zwikszenie wytrzymaoci statycznej testowanych pocze, na kocowy efekt zniszczenia zcza hybrydowego znaczcy wpyw ma powierzchnia zcza klejowego, zwikszona sztywno zczy hybrydowych powoduje, e maj one wiksz niezawodno i trwao jako poczenia
The current manufacturers demands of modern structuralparts of aircrafts requires application of new composite mate-rials with different internal structure, specially introduced tothe material, to modify its properties in order to get: excellentmechanical properties, lightweight, low cost and high securityof structural elements creating whole airplanes. These appli-cations are very important task in case of critical parts of theaircrafts as: elements of engines (e.g. turbine blades), wings,fuselage, joining of critical elements with various techniquesetc. One of the idea of the new composites is to function-alize properties of the material in the form so called func-tionally graded materials FGM (e.g. [1-5]) or by intro-duction layers between material components (e.g. [6-9]) orjoined adherends (e.g. [10-15]) and as TBC covering turbineblades (e.g.[16-19]), etc. Application of adhesives with dif-ferent nano-particles or carbon nano-tubes are other example
to use of modern particle reinforced composites in aerospacetechnology (e.g. [20, 21]). This is the advantage of the ideato use combination of different phases in materials or jointsto create new and stronger composite which guarantee higherdurability and reliability of structural elements in aerospace.
The above ideas are the basis for improvements of joiningtechnologies of structural parts in aerospace. Instead of us-ing single joining technique as: riveting, spot welding, clinch-ing or adhesive bonding a hybrid joining technique (e.g. [15,22]) can be applied by combination of two simple ones, e.g.:riveted-bonding (e.g. [23, 24]), spot welded-bonding (e.g. [25,26], clinched-bonding (e.g. [27-34]), etc. The first applicationof hybrid joints, one of them being adhesive bonding, was in aRussian aircraft construction from 1960 , and it was devel-oped later on the Antonov AN-74 airplane, were a resistancespot welding was combined with the adhesive bonding.
In the paper we will review currently applied different hy-brid joining techniques. The basic idea is to strengthen simple
LUBLIN UNIVERSITY OF TECHNOLOGY, 20-618 LUBLIN, 40 NADBYSTRZYCKA STR., POLAND RZESZW UNIVERSITY OF TECHNOLOGY, 35-959 RZESZW, 8 POWSTANCW WARSZAWY STR., POLAND
Unauthenticated | 126.96.36.199Download Date | 5/12/13 7:24 PM
joining technology by introduction additional adhesive layerbetween adherends, which have many positive effects, like: ahigher static strength, improved fatigue strength, removing ofsealing operations, better corrosion resistance.
The own experimental investigations done with: 1)rivet-adhesive bonded, 2) spot welding adhesive and 3)clinch-adhesive bonded joints confirm the significant improve-ment of mechanical properties of hybrid joints in comparisonto simple one.
The paper describes details of numerical model by appli-cation of FEA for proper characterisation of the mechanicalresponse of these complex hybrid joints. The models incor-porate description of the technological process of the jointcreation (i.e. press forming of the clinch) as well as differ-ent aspects of damage processes which should be applied forfull description of the degradation both: adhesive layers andadherends.
The received results lead to general conclusion that thehybrid joining significantly increases mechanical response ofthe joint, particularly as for load capacity.
2. Rivet-adhesive bonded joints
Let us consider the hybrid Double Lap Joints (DLJ) madeof steel strips adhesive bond layer reinforced by a rivet. Therivet forming process introduces an initial compressive stressto the joint, making the hybrid joint non-symmetric in thethickness direction. The mechanical response of this DLJ wasanalysed in three steps: starting from a simple mechanical rivetjoint, further from a simple adhesive joint and finally byanalysis of the hybrid joint.
The experimental testing included the application of the3-D Digital Image Correlation (DIC) system ARAMIS inorder to monitor the displacements distribution during thejoint testing up to final failure. A numerical modelling wasperformed by Finite Element Analysis (FEA) and softwareABAQUS 6.6. It included the modelling of the rivetingprocess, degradation of the adhesive layer by application ofa Cohesive Zone Model (CZM) and fracture of the alumini-um rivet, similar to . The stress concentrations in differentparts of the joint due to different reasons (riveting process,mechanical loading) were investigated.
2.1. Experimental tests
The samples were prepared from two different kinds ofsteel sheets with a Youngs modulus equal to Es = 210 GPa,and Poissons ratio = 0.3. The steel used for the middle partof DLJ (3 mm thickness) was much stronger in comparison tothat used for the 2 external thinner sheets (1.5 mm thickness).
The rivets, made of aluminium alloy having the Youngsmodulus equal to Er = 70 GPa, whereas Poissons ratio isequal to = 0.3. The mandrel was made of steel. The exert-ed force by the mandrel for the single rivet during formingprocess was equal to Fr = 2 kN.
The adhesive used for the DLJ was the heat curing epoxyadhesive Hysol 9514 (Loctite, Ireland). In order to get max-imum tensile and shear strengths, the specimens were keptin the curing temperature 150C for 30 min, according to
producer recommendation. The shear strength was equal tomax = 45 MPa, whereas tensile strength max = 44 MPa(data supplied by the manufacturer).
Fig. 1. Load-displacement curves for the riveted joints, the adhesivejoints and the hybrid joints
The specimens were subjected to tensile loading usingthe ZWICK Z-100 testing machine at a crosshead displace-ment rate of 2 mm/min. Experimental results for the wholeprogram with the three types of specimens are presented inFig. 1. The steel parts joined mechanically by the rivet exhibita relatively week strength. This is due to the fact that the rivetwas made of aluminium alloy, having not high shear strengthlimit. The shape of the force-displacement diagram is in thefirst stage a linear behaviour, then yielding of steel strips takesplace and finally crack propagation in the adhesive layers (aftermaximum load) in the most efforted zone of the joint started.
The adhesive joint with Hysol 9514 was extremely ef-fective and tough, i.e. the strength of the joint is almost oneorder of magnitude higher in comparison to the rivet joints.The shape of the force-displacement curve is characteristic, i.e.after the first linear part, the curve reaches the local maximumat which the adhesive layers start to fail (damage initiation cri-terion is satisfied in the most efforted parts of the joint). Then,the bonding area load starts to reduce. Therefore, one can ob-serve a local small decrease of the force and then stabilisationcorresponding to further gradual development of failure zonesin adhesive layers, followed by almost linear increase up tothe maximum load.
The hybrid joints have the same geometry as the sim-ple joints. The adhesive was applied on the cleaned steel ad-herends and then the joint was reinforced by a simple rivet.The whole joint was cured at 150C for 30 min. The averagedthickness of the adhesive, measured on the specimen, wasequal to 0.2 mm. The force-displacement curves of the hybridjoints are similar to those of the adhesive joints. However, onecan observe an increase of the failure load due to the presenceof the rivet and synergy between the adhesive and the rivet.Moreover, a significant increase of the displacement at failureis observed for the hybrid joint. Failure takes place at the twobonding interfaces and the rivet.